 Nano Express
 Open Access
 Published:
Localized Surface Plasmon Resonance Dependence on Misaligned Truncated Ag Nanoprism Dimer
Nanoscale Research Letters volume 12, Article number: 430 (2017)
Abstract
Misaligned edgetoedge dimers are the common products during the preparation of Ag nanoprism dimers using selfassembly method. However, in the selfassembly method, Ag nanoprisms are easily truncated because they are easy to oxidize in an acidic environment. In this work, modeling a truncated Ag nanoprism on a misaligned edgetoedge dimer provides a better understanding of the effects of the truncation and misalignment on localized surface plasmon resonance (LSPR) of the dimer. The resonant wavelength and intensity of the dimer are flexibly modulated by changing the misalignment length of the dimer. As the misalignment length increases, a stronger peak at the shorter wavelength and a weaker one at the longer wavelength are observed. The resonant wavelengths and intensities of the two peaks are also flexibly tuned by adjusting the truncated length of the Ag nanoprism in the dimer. The results are numerically demonstrated based on the finite element method (FEM) and show promising potential for nanoswitch, multichannel tunable biosensor and other nanodevice applications.
Background
Silver and gold nanoparticles have attracted extensive attentions due to their unique optical properties which originate from their localized surface plasmon resonance (LSPR) effects. The conduction electrons in these nanoparticles collectively oscillate with the incident light causing an enhanced electric field that is localized around the surface of the nanoparticle [1, 2]. The LSPR effect of nanoparticles can be modulated by changing the nanoparticle’s size, shape, material, and the surrounding environment [3–5]. Among the numerous nanoparticles, nanoprisms (NPs) have attracted the most attention due to their anisotropic geometrical properties and tunable LSPR properties [6–8]. Because of the anisotropic geometrical properties, oscillating charges on the surface tend to accumulate around the NP’s tips making the localized electric field around NP more enhanced than in isotropic nanoparticles [9]. The LSPR properties of NP are usually divided into inplane dipolar resonance, inplane quadrupolar resonance, and outofplane dipolar resonance. The inplane dipolar resonance shows a redshift effect with increasing the edge length of NP [10, 11].
As two nanoparticles are brought close to each other, the enhanced electric field concentrates in the gap of the dimer. This phenomenon is known as hot spot effect which originates from the LSPR coupling effect between the nanoparticles. The dimers with remarkable hot spot effects can be easily prepared by ebeam lithography [12], nanosphere lithography [13], and selfassembly method [14, 15]. For the selfassembly method, metal nanoparticles with specific geometries are linked through the molecules with particular groups. Therefore, the gap in the dimer is as narrow as the molecular chain length. This further reduces the gap between two nanoparticles and causes a more remarkable hot spot effect [16–18].
The hot spot effect of the NP dimer as a typical dimer has been extensively studied, but most studies about the NP dimers concentrate on the tiptotip geometry [19–23]. However, during preparation process of the tiptotip dimer through the selfassembly method, there is a wide existence of NP dimers with edgetoedge geometries [15]. The selfassembly method often causes a randomly misaligned effect for the NP dimers. The randomly misaligned edgetoedge Au NP dimers with the broken symmetry can induce a novel optical property [24]. This result indicates that the double resonances can be switched by modulating the misalignment length of the dimer. The resonant positions can be tuned by changing the gap length and the thickness of Au NP. Due to the sensitivity of optical properties on the structural parameters, this finding paves a promising way for developing nanoswitches, nanomotors, nanorulers, and dualchannel biosensors. However, because of the inertia of the gold atom, the structural parameters of Au NP dimers are usually fixed once they are prepared.
Because Ag is easily oxidized, the tips of the Ag NP can be easily etched in the process of its preparation. This results to Ag NP transforming into an Ag truncated nanoprism (TNP). The change of the structural symmetry originating from the truncation effect induces some novel optical properties [8, 25]. The truncation effect can be introduced in the misaligned edgetoedge Ag NP dimer to obtain a tunable device with novel optical properties. Here, effects of the truncation and misalignment on the LSPR edgetoedge Ag TNP dimers are studied using FEM.
Methods
Structural Model of Misaligned Truncated Ag Nanoprism Dimer
The structural model used in the calculations is shown in Fig. 1. Ag NPs used in the selfassembly method are usually prepared by the seedinduced growth method: its edge length is flexibly modulated by controlling the reaction conditions and keeping the thickness constant [26]. In this paper, the thickness of Ag NP is kept constant at T = 8 nm. The Ag NP edgetoedge dimers are assumed to be prepared by the selfassembly method; therefore, the gap length in this dimer (G) has a specific molecular length G = 2 nm.
The misaligned edgetoedge dimer consists of two identical Ag TNPs with the following dimensions, edge length (L), misalignment length (l _{1}), and truncated length (l _{2}). The tips of Ag NP are cut off along a straight line with the initial edge length L = 130 nm and truncated length l _{2} = 10 nm. To study the effect of the misalignment, a misalignment ratio R = l _{1}/L of Ag TNP dimer is varied from 0 to 1.5. As R approached 0 or 1, the Ag TNP dimers with the increased truncated length were modeled to study the influence of the truncation effect. Ag TNP transforms to a hexagonal nanoplate (HNP), as the edge length of Ag HNP (L _{ 1 }) is equal to the truncated length l _{2} = L/3. To further investigate the effect of the truncation and misalignment, Ag HNP dimers with the misalignment ratio R _{ 1 } = l _{1}/L _{ 1 }, ranging from 0 to 3, were simulated.
Finite Element Method for Misaligned Truncated Ag Nanoprism Dimer
FEM method using COMSOL Multiphysics is used to investigate the effect of misalignment length on the LSPR edgetoedge Ag TNP dimer. The relative permittivity for Ag was obtained from the Drude model, ε(ω) = ε _{∞} − ω _{ p } ^{2}/[ω(ω + iγ)], where ε _{∞} = 3.7 is the infinite frequency, ω _{ p } = 1.38 × 10^{16} is the bulk plasma frequency, and γ = 3.72 × 10^{13} is the oscillation damping of electrons [27].
The Ag TNP dimer was modeled on the xy plane at z = 0 with air (n = 1) surrounding it. Using air around the dimer was done to simplify the computation process. The incident light, polarized along the yaxis, was directed normally along zaxis on the Ag TNP surface. Tuning of the wavelength was done between λ = 600 nm to λ = 1100 nm with a step of 4 nm.
Results and Discussion
The extinction crosssection (ECS) intensity distribution map of the Ag TNP dimer showing variation between the wavelength and R was firstly calculated to investigate effect of the misalignment length on the LSPR. Figure 2 shows the ECS intensity distribution color map of the Ag TNP dimer. As shown in Fig. 2, the Ag TNP dimer with R = 0 displays two peaks with equal intensities. When R is equal to 1, the shorter wavelength peak, labeled as peak 1, is strong and shows a blueshift effect. For the longer wavelength, labeled as peak 2, the intensity decreases and shows a blueshift effect. As R is increased from 0 to 1, the resonant wavelength of peak 1 initially decreases and then slightly stabilizes. Meanwhile, its intensity gradually increases. It is worth noting that peak 1 decreases abruptly when R changes from 0 to 1/8. This is because the disappearance of the higherorder LSPR mode. The resonant wavelength of peak 2 first increases and then decreases, but its intensity decreases throughout.
Peak 1 in Fig. 2a strengthens further as R increases from 1 to 1.5 and its resonant wavelength is kept unchanged. Moreover, peak 2 continuously decreases until it disappears while its resonant wavelength decreases throughout. As R reaches 1.5, the double peaks degenerate into a single peak with a resonant wavelength equal to that of the Ag TNP monomer. When R is large than 1, the LSPR coupling interaction between Ag TNPs is extremely weak. In Fig. 2b, peak 2 plays the dominant role in ECS spectrum when R < 0.5 (the blue region) whereas peak 1 dominates when R > 0.5 (the yellow region). Therefore, the two peaks can be switched on or off by modulating the misalignment length of the dimer.
The electric field distributions of Ag TNP dimers for different values of R are shown in Fig. 3. The geometrical configuration of the Ag TNP dimer changes as R varies from 0 to 1.5. When R is equal to 0, the Ag TNP dimer possesses the edgetoedge geometry. As R reaches to 1, the configuration changes into the tiptotip geometry, and as R increases further, the configuration turns an abnormal tiptotip geometry. In Fig. 3a, the enhanced electric fields are localized at the center and two ends of the gap, so for R = 0, peak 1 is a higherorder LSPR mode. When R is larger than 0, the higherorder LSPR mode disappears and the structural symmetry of the dimer is broken. Then peak 1 can be attributed to the antisymmetric mode from the LSPR coupling interaction between Ag truncated nanoprisms in the dimer shown in Fig. 3b–d. The electric fields mainly distribute around the lateral tips away from the gap in the Ag TNP dimer. When R is large enough, the electric field distributions of Ag TNPs in the dimer are similar to that of the Ag TNP monomer as shown in Fig. 3h. Figure 3e–g show that peak 2 can be attributed to the symmetric mode from the LSPR coupling interaction between Ag truncated nanoprisms in the dimer. The enhanced electric fields are mainly localized in the gaps. The results show that the two peaks can be turned on or off by modulating the LSPR coupling interaction between Ag TNPs in the dimer. When R is equal to 0, Ag TNP dimers for the two peaks possess huge enhanced electric fields (above 900 V/m) in the gap. The enhancement effect of the surrounding electric field of the Ag TNP dimers weakens as R increases. This means that the misalignment effect will weaken the hot spot effect of Ag TNP dimer, if R increases and the enhanced electric field distribution will shift from the gap to the lateral tips of Ag TNP in the dimer.
To investigate the effect of the truncation on the switching, the truncated lengthdependent ECS resonant wavelength and intensity spectra of the Ag TNP dimers are simulated and shown in Fig. 4 (for R = 0, 1). When the truncated length l _{2} is 43.3 nm and L = 130 nm, Ag TNP turns into Ag HNP. As shown in Fig. 4a, peak 1 abruptly decreases from the initial strong state and then stabilizes in a weak state as l _{2} is increased when R = 0. This is because the higherorder LSPR mode corresponding to peak 1 at the same R value no longer exists in the gap as the gap length decreases (i.e., as l _{2} increases). The origin of peak 1 changes from the higherorder LSPR mode to the antisymmetric mode of the LSPR coupling interaction as the truncated length increases. When R equals to 0 or 1 as shown in Fig. 4, the resonant wavelengths of the two peaks decrease throughout. As shown in Fig. 4b, peak 2 gradually fades as l _{2} increases to a specific value, the double peaks degenerate to a single peak. Similarly, this is due to the symmetric mode from the LSPR coupling interaction weakening as the interval between the two Ag TNPs increases (i.e., as l _{2} increases). This means that the switching effect of the Ag TNP dimer can be flexibly modulated by changing the truncated length originating from the easytooxidize features of Ag.
When the truncated length increases to a critical value, Ag TNP in the dimer transforms into Ag HNP. The edge length of Ag HNP L _{ 1 } is 43.3 nm. Figure 5 shows the ECS intensity distribution map of Ag HNP dimers versus R _{1} and wavelength. Here, the wavelength of the incident light ranges from 500 to 900 nm. For the Ag HNP edgetoedge dimer, a change of the misalignment length (l _{1}) also causes the variations of two peaks in its ECS spectrum. With increasing the misalignment ratio R _{ 1 } = l _{1}/L _{ 1 }, the switching effect of the Ag HNP edgetoedge dimer is more remarkable than the Ag TNP dimer. Peak 2 originating from the symmetric mode of the LSPR coupling interaction quickly fades in the ECS spectrum with the two Ag HNPs moving away from each other (R _{ 1 } > 1) as shown in Fig. 5. Peak 1 originates from the antisymmetric mode from the LSPR coupling interaction between Ag HNPs and gradually occupies the dominant role. The intensity ratio of peak 2 to peak 1 for the Ag HNP dimer is obviously larger than that of the Ag TNP dimer. Compared with the ECS spectrum of the Ag TNP dimer, the Ag HNP dimer possesses a single peak configuration which also can be switched by changing the misalignment length. This is further evidence that Ag NP edgetoedge dimers with different truncated length possess a misalignmentrelated switching effect.
Conclusions
In summary, the LSPR effects of Ag TNP misaligned edgetoedge dimers have been studied using FEM. The ECS spectrum of Ag TNP dimer possesses two peaks, which can be switched on or off by modulating the misalignment length. When R is less than 0.5, the longer wavelength peak plays the prominent role in the ECS spectrum. As R grows larger than 0.5, the shorter wavelength peak occupies the dominant role. Due to the truncation effect, the resonant wavelengths of the two peaks can be flexibly modulated by changing the truncated length. When the truncated length increases to a specific value, Ag TNP transforms into Ag HNP. The double peaks degenerate to a single peak, and the peaks of the Ag HNP dimer also can be switched by changing the misalignment length. The calculated results indicate that Ag TNP misaligned edgetoedge dimers pave the way for a promising surfaceenhanced Raman spectrum, nanoswitch, multichannel tunable biosensor, other nanodevices, etc.
Abbreviations
 ECS:

Extinction crosssection
 FEM:

Finite element method
 G :

Gap length
 HNP:

Hexagonal nanoplate
 L :

Edge length
 l _{1} :

Misalignment length
 l _{2} :

Truncated length
 LSPR:

Localized surface plasmon resonance
 NP:

Nanoprism
 R :

Misalignment ratio
 T :

Thickness
 TNP:

Truncated nanoprism
References
Nien LW, Lin SC, Chao BK, Chen MJ, Li JH, Hsueh CH (2013) Giant electric field enhancement and localized surface plasmon resonance by optimizing contour bowtie nanoantennas. J Phys Chem C 117(47):25004–25011
Liu Y, Huang CZ (2013) Screening sensitive nanosensors via the investigation of shapedependent localized surface plasmon resonance of single Ag nanoparticles. Nanoscale 5(16):7458–7466
Liu Y, Song F, Zhang J, Lv Z, Liu J, Yu Y, Zhao H, Wang H (2013) Tunable local surface plasmon resonance in liquidcrystalcoated Ag nanoparticles. Phys Lett A 377(16–17):1199–1204
Le Thi Ngoc L, Jin M, Wiedemair J, van den Berg A, Carlen ET (2013) Large area metal nanowire arrays with tunable sub20 nm nanogaps. ACS Nano 7(6):5223–5234
Personick ML, Langille MR, Zhang J, Wu J, Li S, Mirkin CA (2013) Plasmonmediated synthesis of silver cubes with unusual twinning structures using short wavelength excitation. Small 9(11):1947–1953
Millstone JE, Hurst SJ, Metraux GS, Cutler JI, Mirkin CA (2009) Colloidal gold and silver triangular nanoprisms. Small 5(6):646–664
Shuford KL, Ratner MA, Schatz GC (2005) Multipolar excitation in triangular nanoprisms. J Chem Phys 123(11):114713
Jin R, Cao Y, Mirkin CA, Kelly KL, Schatz GC, Zheng JG (2001) Photoinduced conversion of silver nanospheres to nanoprisms. Science 294:1091–1093
Aherne D, Ledwith DM, Gara M, Kelly JM (2008) Optical properties and growth aspects of silver nanoprisms produced by a highly reproducible and rapid synthesis at room temperature. Adv Funct Mater 18(14):2005–2016
Yang P, Portalès H, Pileni MP (2009) Identification of multipolar surface plasmon resonances in triangular silver nanoprisms with very high aspect ratios ysing the DDA method. J Phys Chem C 113(27):11597–11604
Hermoso W, Alves TV, de Oliveira CCS, Moriya EG, Ornellas FR, Camargo PHC (2013) Triangular metal nanoprisms of Ag, Au, and Cu: modeling the influence of size, composition, and excitation wavelength on the optical properties. Chem Phys 423:142–150
Kim S, Jin J, Kim YJ, Park IY, Kim Y, Kim SW (2008) Highharmonic generation by resonant plasmon field enhancement. Nature 453(7196):757–760
Haynes CL, Van Duyne RP (2001) Nanosphere lithography: a versatile nanofabrication tool for studies of sizedependent nanoparticle optics. J Phys Chem B 105(24):5599–5611
Gao B, Arya G, Tao AR (2012) Selforienting nanocubes for the assembly of plasmonic nanojunctions. Nat Nanotechnol 7(7):433–437
Gao B, Alvi Y, Rosen D, Lav M, Tao AR (2013) Designer nanojunctions: orienting shaped nanoparticles within polymer thinfilm nanocomposites. Chem Commun 49(39):4382–4384
Li W, Camargo PH, Au L, Zhang Q, Rycenga M, Xia Y (2010) Etching and dimerization: a simple and versatile route to dimers of silver nanospheres with a range of sizes. Angew Chem 49(1):164–168
Kessentini S, Barchiesi D, D’Andrea C, Toma A, Guillot N, Di Fabrizio E, Fazio B, Maragó OM, Gucciardi PG, Lamy de la Chapelle M (2014) Gold dimer nanoantenna with slanted gap for tunable LSPR and improved SERS. J Phys Chem C 118(6):3209–3219
Ci X, Wu B, Song M, Liu Y, Chen G, Wu E, Zeng H (2014) Tunable Fano resonances in heterogenous AlAg nanorod dimers. Appl Phys A 117(2):955–960
Lin TR, Chang SW, Chuang SL, Zhang Z, Schuck PJ (2010) Coating effect on optical resonance of plasmonic nanobowtie antenna. Appl Phys Lett 97(6):063106
Grzeskiewicz B, Ptaszynski K, Kotkowiak M (2014) Near and farfield properties of nanoprisms with rounded edges. Plasmonics 9:607–614
Guo H, Meyrath TP, Zentgraf T, Liu N, Fu L, Schweizer H, Giessen H (2008) Optical resonances of bowtie slot antennas and their geometry and material dependence. Opt Express 16(11):7756–7766
Hatab NA, Hsueh CH, Gaddis AL, Retterer ST, Li JH, Eres G, Zhang Z, Gu B (2010) Freestanding optical gold bowtie nanoantenna with variable gap size for enhanced Raman spectroscopy. Nano Lett 10(12):4952–4955
Rosen DA, Tao AR (2014) Modeling the optical properties of bowtie antenna generated by selfassembled Ag triangular nanoprisms. ACS Appl Mater Interfaces 6(6):4134–4142
Zhang CH, Zhu J, Li JJ, Zhao JW (2015) Misaligndependent double plasmon modes “switch” of gold triangular nanoplate dimers. J Appl Phys 117(6):063102
Fischer H, Martin OJF (2008) Engineering the optical response of plasmonic nanoantennas. Opt Express 16(12):9144–9154
Goebl J, Zhang Q, He L, Yin Y (2012) Monitoring the shape evolution of silver nanoplates: a marker study. Angew Chem 51(2):552–555
Park J, Kim H, Lee B (2008) High order plasmonic Bragg reflection in the metalinsulatormetal waveguide Bragg grating. Opt Express 16(1):413–425
Funding
This study is financially supported by the National Natural Science Foundation of China (No. 11374074, 61308069) and the National Basic Research Program of China (No. 2013CB328702).
Authors’ Contributions
HYA, XJ, and XS conceived the idea. HYA, EO, PL, and XS calculated the results and made the conclusions. HYA, EO, and SL contributed to the preparation and revision of the manuscript. All the authors read and approved the final manuscript.
Competing Interests
The authors declare that they have no competing interests.
Publisher’s Note
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Author information
Authors and Affiliations
Corresponding author
Rights and permissions
Open Access This article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
About this article
Cite this article
Yang, H., Owiti, E.O., Jiang, X. et al. Localized Surface Plasmon Resonance Dependence on Misaligned Truncated Ag Nanoprism Dimer. Nanoscale Res Lett 12, 430 (2017). https://doi.org/10.1186/s1167101720624
Received:
Accepted:
Published:
DOI: https://doi.org/10.1186/s1167101720624
Keywords
 LSPR
 Misalignment
 Truncation
 Ag Nanoprism dimer